Examples of nanoparticles stabilized by imidazolium based ILs.
For over a decade, ionic liquids (ILs) have attracted enormous attention from scientists across the globe. The history of these compounds traces back to 1914 where the inception of the first IL with a melting point of 12°C was made. Years later, a progression of the remarkable related compounds have been discovered. Out of many analogous compounds realized from time to time, the imidazolium class of ionic liquid is the most studied because of their air and moisture stability. The physicochemical properties of ILs differ significantly depending on the anionic/cationic species and alkyl chain length. ILs have found application in many scientific fields the most recent being good solvents and stabilizing agents in the nanomaterial synthesis. Studies have showed that ILs not only stabilize as synthesized nanomaterials but also provide environmentally green routes towards nanomaterials engineering.
- ionic liquids
- green solvent
- imidazolium-based ionic liquid
- capping agents
Nanomaterials have penetrated numerous multidisciplinary research fields in both science and engineering domains, leading to the development of next generation products which have already made a debut in the commercial marketplace . To date, synthetic methods and protocols remain of fundamental importance in accessing and harnessing unique properties of materials as their particle sizes approach the nanometer size regime. Suspended nanomaterials are usually desired due to their suitability with various applications and they are easily prepared from chemical approaches. These approaches provide opportunities in tailoring and tuning the properties of the nanomaterials to suit desired applications by tweaking reaction parameters. Two main reaction parameters have received attention, namely, (1) the type and nature of the precursor/s [2, 3, 4], as well as (2) the nature of the solvent used during and after completion of the fabrication process [5, 6, 7]. Nanomaterials have, however, received their share of potential negative implications on the environment and its inhabitants . Thus, efforts in devising eco-friendly reaction protocols have been seen as a proper response. In this chapter, imidazolium-based ILs are reviewed as green solvents over conventional organic solvents for use in the synthesis of nanomaterials.
The general use of conventional organic solvents in various laboratory and industrial processes has presented issues over the years. For example, in pharmaceutical production, the high energy consumption (
Ionic liquids (ILs) are generally molten salts composed of organic cations and organic or inorganic anions, with characteristic melting points below 100°C. They possess unique physicochemical properties such as low viscosity , negligible vapor pressure , non-flammability , good thermal and chemical stability , high ionic conductivity , and tunable solubility for both organic and inorganic molecules. They are thus regarded as environmentally-friendly and may lead to the formation of novel materials that have never been achieved by conventional solvents or even water. ILs are normally characterized by their cationic components of which imidazolium , pyridinium , ammonium , pyrrolidinium , piperidinium  and phosphonium  cations with different alkyl chain lengths being the most common (Figure 1). Examples of some commonly used anions are shown in Figure 2. ILs can be classified further into groups,
The complexity and suitability of ILs in various applications have been debated over the years. Many questions have been asked about the complexity (and sometimes even the simplicity) associated with the usefulness of ionic liquids in various fields of science specifically their use as solvents. However, the hybrid ionic nature of ILs and the resultant intermolecular interactions give rise to a complex set of phenomena, creating an area of study that is both interesting and challenging. Furthermore, they have been extensively studied and researched as potential solvents for inorganic nanomaterial synthesis, organic chemical reactions, polymer synthesis and electrochemical applications [34, 35, 36, 37, 38]. Thus, the aim of this chapter is to rather highlight the recent developments and breakthroughs in exploiting the interesting physicochemical properties of ILs in the world of nanomaterials. The scope will be restricted to the use of room temperature ILs as green solvents for the synthesis and stabilization of inorganic nanomaterials. Prior to this, the physicochemical properties of ILs will be briefly outlined.
2. Physicochemical properties of ILs
The physicochemical properties of ILs (e.g. viscosity, melting point, hydrophobicity, solvation, and catalytic activity) can be tuned by changing the alkyl chain length in the cationic and/or the anion groups [39, 40]. Task specific or targeting ILs can be synthesized by careful choice and combination of the cationic and anionic groups, to suit a specific application. A catalysis-themed review article by Sheldon , for example, outlines the potential use of ILs as both reaction media and catalysts. The former was, however, found to have a profound effect on the catalytic activities and selectivity.
Greater van der Waals forces and hydrogen bonding are typical attributes of materials exhibiting high viscosities [41, 42]. Generally, ILs are highly viscous than most common molecular solvents, with viscosity ranging between 10 and 500 mPa s at room temperature . The cation structure influences the IL viscosity with minimal values reported for ethylmethylimidazolium, EtMeIm+ ILs. Furthermore, EtMeIm+ ILs have adequate side chain mobility and low molecular weight. Generally, the viscosity of ILs increases with alkyl chain length and degree of fluorination . Anions also have an influence over the viscosity of ILs, e.g. [BMIm]PF6 = 312 mPa , [BMIm]BF4 = 154 mPa  and [BMIm]TF2N = 52 mPa .
ILs have relatively good ionic conductivities compared to organic solvents and electrolytic systems (up to about 10 mS cm−1) . Susan et al.  first demonstrated that fused ammonium salts can be used as proton conductors in polymer membrane fuel cells . According to Greaves et al. , “ionic conductivity is a transport property and is governed by the degree of dissociation of the ions, viscosity, ion mobility, and ionic charge”. These aforementioned factors depend on the effective ion sizes and shapes. Furthermore, ionic conductivity of ILs is inversely proportional to viscosity and molar volume .
2.3. Melting point
The general description of ILs is that of ionic salts that are in a liquid phase below an arbitrary temperature of 100°C; the majority of ILs are solids at standard room temperature. From a practical point of view, ILs are desirable in their molten state e.g. transportation of ILs across multiple unit operations in industrial applications is most effective in their liquid phase. ILs exhibiting of significantly lower melting points or “room temperature ILs” (Tm < 25°C) are critically important to researchers searching for new industrial applications . One main reason for their demand is their usage as solvents or absorbents for separation tasks involving selective dissolution of solutes in gas (e.g. CO2), liquid (e.g. toluene), or solid (e.g. cellulose) states. They are also widely considered as liquid solvents to promote chemical reactions .
ILs are generally denser than water, with values ranging from 1 to 1.6 g cm−3 and their densities decrease with increase in alkyl chain length in the cation . For example, ILs composed of substituted imidazolium-type cations and CF3SO3− anion display densities of 1.39, 1.33, 1.29 and 1.27 g cm−3 for [EMIm]+, [EEIm]+, [BMIm]+ and [BEIm]+, respectively . The densities of ILs are also affected by the nature of anions, e.g. the densities of 1-butyl-3-methylimidazolium-type ILs with different anions, such as BF4, PF6, TFA and Tf2N in literature are recorded to be 1.12, 1.21, 1.36 and 1.43 g cm−3, respectively [44, 53]. The order of increasing density with respect to anions is: [CH3SO3]− ≈ [BF4]− < [CF3CO2]− < [CF3SO3]− < [C3F7CO2]− < [(CF3SO2)2N]−, in Ref. .
2.5. Electrochemical window
The electrochemical window allows ILs to be used in the electrodeposition of semiconductors and metals. The electrochemical window, by definition, is the electrochemical potential range over which the electrolyte is neither reduced nor oxidized at an electrode. Thus, the magnitude of the electrochemical value determines the solvent’s electrochemical stability. The electrodeposition of elements and compounds in water is limited by its low electrochemical window of only about 1.2 V. On the contrary, ILs have significantly larger electrochemical windows, for example, 4.15 V for [BMIm]PF6 at a platinum electrode, 4.10 V for [BMIm]BF4 and 5.5 V for [BMP]Tf2N at a glassy carbon electrode [54, 55]. Generally, the wide electrochemical windows of ILs have opened the new horizon for the electrodeposition-assisted synthesis of metals and semiconductors at room temperature, which were previously achieved only from molten salts at high reaction temperatures.
2.6. Thermal stability
Most solvents are thermally stable at high temperatures only for short durations; long time exposure habitually leads undesirable decomposition . On the other hand, ILs are known to be thermally stable up to 450°C. Their thermal stability is limited by the strength of their hydrocarbon bonds . It is common knowledge that ILs with larger proton transfer energies prematurely decompose before reaching their boiling points with varying decomposition temperatures ranging between 100 and 360°C . Protic ILs with a bis(trifluoromethane) sulfonamide anion and alkylammonium, imidazolium and a range of other heterocyclic cations are identified as the most stable ILs due to their bond strength resulting from resonance stabilization . Specifically, ILs such as 1-ethyl-3-methyl-imidazolium tetrafluoroborate, 1-butyl-3-methyl-imdazolium tetrafluoroborate and 1,2-dimethyl-3-propyl imidazolium bis(trifluorosulfonyl)imide are thermally stable up to 445, 423 and 457°C, respectively . The anionic components is known to predominantly contribute to the thermal stability of the ILs over the cationic counterparts. Furthermore, the hydrophilicity of the anions decreases thermal stability of the ILs .
3. Imidazolium-based ionic liquids
ILs with the 1,3-dialkylimidazolium cation are by far the most studied class of ILs due to their interesting properties. The class can interact with various chemical species, as they offer hydrophobic or hydrophilic regions and a high directional polarizability. The structural organization of these solvents can be used as ‘entropic drivers’ for spontaneous, well-defined, and prolonged ordering of nanoscale structures. Certainly, the unique combination of flexibility towards other molecules (and phases) with strong hydrogen-bond-driven structures make ILs potential key tools in the preparation of a new generation of chemical nanostructures .
4. Imidazolium-based ionic liquids in nanomaterial synthesis
Generally, ILs have chemical attributes such as non-volatility, negligible vapor pressure and most importantly, high thermal stability . The majority of the fabrication protocols require heat to be applied, thus controlling both nucleation and growth rates to ensure monodispersity in suspended nanomaterials . Functional groups of organic solvents determine stability and coordination mode towards nanomaterials . Similarly, the composition of the ILs (combination of organic cation with organic or inorganic anion) play a major role in determining the final chemical attributes. The early reports have demonstrated ILs as dual-action reagents, i.e. as both solvent media and template or structure/shape-directing agent [61, 62]. Furthermore, the recovery of ILs after completion of nanomaterials synthesis strengthens their classification as eco-friendly solvents. The negligible vapor pressure feature enables reactions in ILs to proceed in ambient pressure when subjected to synthetic protocols common for hydro- and solvothermal methods, hence the reactions are rather termed ionothermal synthesis .
In recent years the advantages of incorporating ILs in the synthesis of inorganic nanomaterials have been thoroughly demonstrated, due to their unique physicochemical properties [63, 64]. Several ILS-incorporated methods and protocols have been reported for the fabrication of inorganic nanomaterials. Synthetic reactions, in the presence of ILs, offers nanomaterials to display exceptional and/or unique properties .
4.1. Electrostatic stabilization of nanomaterials by ILs
Ionic compounds such as carboxylates, polyoxoanions and fluorides usually generate double layers between the nanoparticles, thereby introducing repulsive forces between individual nanoparticles. Thus, electrostatic repulsions prevent aggregations and agglomeration of nanoparticles suspended in the solution phase. This type of electrostatic stabilization is sensitive to reaction parameters such as pH, concentration and temperature. This has been demonstrated in metal nanoparticles stabilized by ILs composed of sulfonium, tertiary butyl ammonium, phosphonium and imidazolium moieties . A graphical illustration of this kind of stabilization is shown in Figure 3.
4.2. Steric stabilization of nanomaterials by ILs
Steric stabilization of nanoparticles is another significant parameter. This usually happens through the use of surfactants, alcohols and a variety of polymers/oligomers. These compounds are adsorbed on the nanoparticle’s surface, thereby forming a protective layer . When the nanoparticles are sterically stabilized, their free motion in solution is limited. Furthermore, the thickness of the protective layer has an important role in the stabilization process and greatly depends on the alkyl chain length and nature of the stabilizing agent, where applicable .
4.3. A combination of electrostatic and steric stabilization of nanomaterials by ILs
Both electrostatic and steric stabilization processes can co-exist in the stabilization of nanoparticles in solution phase. Ionic surfactants with long alkyl chains ordinarily provide this type of stabilization. This is mostly achieved through ILs which have polar heads groups which generate electric double layer around the nanoparticle and a lipophilic tail group providing the steric repulsions between nanoparticles . Examples of IL-stabilized nanoparticles are listed in Table 1.
|IL used||NP synthesized||Size (nm)||IL name and reference|
|Al2O3, TiO2, Fe3O4||80–100||1-methacryloyloxypropyl-3-methylimidazolium bromide |
|ZnSe||70–100||1-butyl-3-methylimidazolium methyl sulfate |
|PbS||100||1-n-butyl-3-methylimidazolium hexafluorophosphate |
|CdS, PbS||2–15, 102–160||1-ethyl-3-methylimidazolium methanesulfonate |
|Ni||4.9–5.9||1-alkyl-3-methylimidazolium N-bis(trifluoromethane sulfonyl) |
|Au||140||n-butyltrimethylammonium N-bis(trifluoromethylsulfonyl)imide |
|Ir||2.4–2.6||1-n-butyl-3-methyl trifluoromethane sulfonate |
4.4. Practical examples of imidazolium-based ILs used in the synthesis of nanomaterials
The diversity of ILs presents a challenge is identifying the relationship/trend between their physiochemical properties and morphological (also crystal phase) control of the nanomaterials. It is for these reasons ILs have been used in conjunction with conventional organic solvents to synthesize nanomaterials [68, 74, 75]. Since the influence of ILs on the properties of nanomaterials is not predictable at this stage, there are efforts in conducting investigations for the sake of rather establishing databases. A good example is the work by Duan et al.  where ILs are demonstrated as both solvent and shape-directing agent in the synthesis of γ-AlOOH and well-dispersed NH4Al(OH)2CO3 nanostructures. The same group extended the study on ferric giniite crystals (Figure 4) which revealed interesting photocatalytic behavior which could only be linked to exposed facets of the crystals, as opposed to the surface area . There are reports that have documented evidence of imidazolium-based ILs having acted as capping agents [78, 79]. Zheng and co-workers [79, 80] have given plausible reasons that support capping through interaction modes of imidazolium-based ILs with TiO2 nanoparticles, for example, hydrogen bonding between the positively charged (due to delocalization) position-2 H atom in the imidazole ring with O on the TiO2 surface.
IL-nanomaterial composites have also been reported for use in biological applications, e.g. the study by Alavi-Tabari et al.  demonstrates the use of 1-butyl-3-methylimidazolium tetrafluoroborate IL to form IL-ZnO composites for potential activity enhancement of doxorubicin and dasatinib for breast anticancer remedies. In their study the outcome showed that ZnO-NPs/BMTFB/CPE reveals two different oxidation signals for the simultaneous examination of doxorubicin and dasatinib, which eventually showed a good linear relationship between the oxidation peak current of doxorubicin and its concentration. They concluded that ZnO-NPs/BMTFB/CPE showed good capacity for analysis of doxorubicin and dasatinib in injection and serum samples. Husanu et al.  reported an easy synthetic method focusing on preparing citrate-based ILs which showed a dual-action feature, an ability to act as both capping agents and reducing agents towards the preparation of inorganic nanomaterials.
Although the topic “ILs in the synthesis of nanomaterials” is not of novel origin, the ‘novelty’ is observed where a new class of ILs is prepared through the incorporation of new anionic groups. This subsequently results in the synthesis of nanomaterials bearing desired properties. For example; 3-(hydroxypropyl)-3-methylimidazolium bis(salicylato)borate (OHMimBScB) IL has been used for the covalent grafting of carbon quantum dots via a bottom up approach . Since ILs have strong adsorption capabilities, the surface on the carbon quantum dots was protected against friction, which then improved their stability efficiency in tribological evaluations. Saien and Hashemi  used 1-hexadecyl-3-methyl imidazolium chloride IL as a surfactant to study its interaction with Fe3O4 nanoparticles in a biphasic oil/water system. In a study by Okoli et al.  it was found that the sole use of ILs without additional co-surfactants is capable of producing good quality (monodispersity with narrow size distribution) metal alloy nanoparticles which display enhanced catalytic activities.
A pre-concentration technique based on the use of graphene oxide (GO) functionalized with an IL was established for the determination of Hg traces in water . In this study, the hybrid IL-GO nanomaterial was fabricated by a simple procedure, where the IL used was 1-butyl-3-dodecylimidazolium bromide ([C4C12im]Br). The incorporation of [C4C12im]Br led to high sorption performances on Hg. Furthermore, functionalization of the imidazolium ring with long alkyl chains increased the retention competence of GO for the analyte, consequently providing additional physicochemical properties that were beneficial for the extraction of Hg and its control at trace levels.
Other interesting reports include the use of ILs as a solvent medium in the electrochemical exfoliation of graphite to obtain nanomaterials of significant technological importance i.e. fluorescent carbon nanoribbons, nanoparticles and graphene (Figure 5) . ILs are most suited for this task due to their broad electrochemical window, as well as high dielectric constant necessary to counteract stacking in nanomaterials resulting from van der Waals interactions. Furthermore, imidazolium-based IL-capped carbon quantum dots have been prepared by pyrolysis . Recently, imidazolium-based IL has been used to exfoliate 2D transition metal chalcogenide, WS2 nanosheets . Prechtl et al.  demonstrated the use of ILs as both stabilizing and reducing agents in the preparation of metal nanoparticles from organometallic complexes. Similarly, citrate-modified ILs were recently used to prepare IL-capped Ag nanoparticles .
5. Tuning the properties of nanomaterials (NMs) through the use of IBILs
Stabilization of nanoparticles using different media has been necessary to suit various applications. The medium plays a key role in modifying and tuning the chemical and physical properties of the nanomaterials [91, 92]. Various synthetic routes such as colloidal methods use solvent-mediated chemical procedures to form colloids via self-assembly or other processes related to the tuning of physicochemical properties . The former process usually proceeds via the homogeneous nucleation of particles and subsequent particle growth by condensation, coagulation and arrest of particles (Figure 6).
Imidazolium-based ILs have been reported to improve the electric conductivity of multi-walled carbon nanotubes for electrochemical or electro catalytic applications . Covalent interaction linkage ensures improved oxidation and hydrogenation reactions. Imidazolium-based ILs provide surface stabilization of nanoparticles over a long period of time with insignificant or no change in particle size and size distribution, providing re-usable or recyclability capabilities in applications such as catalysis . Photocatalyst stabilized by imidazolium-based ILs are known to bind strongly and could be easily separated from the reaction mixture without contamination or significant loss in catalytic performance .
Interestingly, small-sized Cu nanoparticles (6.6 nm) have reportedly been synthesized
The type of functional group present in the IBIL determines the mode of interaction with the nanoparticle. Furthermore, tweaking of the reaction parameters has become a common practice to manipulate these interaction modes, thus, enabling particle size and shape-directing capabilities. The chemical structure of 1-ethyl-3-methylimidazolium IL, in the recent study, afforded covalent, coordinate, electrostatic/steric or weak chemisorption interactions via their cations and counter anions (Figure 8) to produce CdS and PbS nanoparticles [70, 98]. The 1-ethyl-3-methylimidazolium IL efficiently produced very small and well dispersed CdS quantum dots in the size range of 2.3–4.3 ± 0.265 nm, attributed to the presence of both cationic and anionic components . Cubic-shaped and highly crystalline PbS nanoparticles in the particle size range of 64 ± 18 nm were synthesized using the same 1-ethyl-3-methylimidazolium IL (Figure 8) .
Ionic liquids (ILs), imidazolium-based ILs (IBILs) in particular, have been exploited in various applications including its use as both reactants and stabilizing agents in the synthesis of functional nanomaterials. The remarkable merit of IBILs and ILs in general is their diversified design which involves a vast selection of cations and anions species. The physicochemical properties of ILs play a major role in improving, modifying and tuning important properties of nanomaterials such as particle size and morphology to suit various applications. Interestingly, the physicochemical properties of ILs further provide unique stability for nanomaterials, which guarantees longer shelf life. In addition, ILs are known to be less toxic, thus enabling them to be used as alternative eco-friendly candidates in various studies as means of applying green chemistry principles. The properties of ILs change with cation/anion composition and there is currently no model to predict its interactions and subsequent influence on the properties of nanomaterials. Hence, an increasing interest observed in evaluating ILs as both reactants and stabilizing agent in the synthesis of different classes of nanomaterials.
Z. Tshemese, S. Mlowe, N. Revaprasadu and S.C. Masikane wishes to thank the National Research Foundation—South Africa (NRF) for financial support.
Conflict of interest
We declare no conflict of interest.
Vance ME, Kuiken T, Vejerano EP, McGinnis SP, Hochella MF Jr, Rejeski D, Hull MS. Nanotechnology in the real world: Redeveloping the nanomaterial consumer products inventory. Beilstein Journal of Nanotechnology. 2015; 6:1769
Kumar S, Nann T. Shape control of II–VI semiconductor nanomaterials. Small. 2006; 2(3):316-329
Tian L, Yao Tan H, Vittal JJ. Morphology-controlled synthesis of Bi2S3 nanomaterials via single-and multiple-source approaches. Crystal Growth and Design. 2007; 8(2):734-738
Wooten AJ, Werder DJ, Williams DJ, Casson JL, Hollingsworth JA. Solution-liquid-solid growth of ternary Cu-In-Se semiconductor nanowires from multiple- and single-source precursors. Journal of the American Chemical Society. 2009; 131(44):16177-16188
Green M. The nature of quantum dot capping ligands. Journal of Materials Chemistry. 2010; 20(28):5797-5809
Garnweitner G, Niederberger M. Organic chemistry in inorganic nanomaterials synthesis. Journal of Materials Chemistry. 2008; 18(11):1171-1182
Al-Salim N, Young AG, Tilley RD, McQuillan AJ, Xia J. Synthesis of CdSes nanocrystals in coordinating and noncoordinating solvents: Solvent's role in evolution of the optical and structural properties. Chemistry of Materials. 2007; 19(21):5185-5193
Buzea C, Pacheco I, Robbie K. Biointerphases 2. MR17. 2017; 2(4):17-71
Slater CS, Savelski M. A method to characterize the greenness of solvents used in pharmaceutical manufacture. Journal of Environmental Science and Health Part A. 2007; 42(11):1595-1605
Rundquist EM, Pink CJ, Livingston AG. Organic solvent nanofiltration: A potential alternative to distillation for solvent recovery from crystallisation mother liquors. Green Chemistry. 2012; 14(8):2197-2205
Ghandi K. A review of ionic liquids, their limits and applications. Green and Sustainable Chemistry. 2014; 4(1):44-53
Seddon KR. Ionic liquids for clean technology. Journal of Chemical Technology and Biotechnology. 1997; 68(4):351-356
Earle MJ, Esperança JM, Gilea MA, Lopes JNC, Rebelo LP, Magee JW, Seddon KR, Widegren JA. The distillation and volatility of ionic liquids. Nature. 2006; 439(7078):831-834
Ye C, Liu W, Chen Y, Yu L. Room-temperature ionic liquids: A novel versatile lubricant. Chemical Communications. 2001; 21:2244-2245
He Z, Alexandridis P. Nanoparticles in ionic liquids: Interactions and organization. Physical Chemistry Chemical Physics. 2015; 17(28):18238-18261
Noda A, Hayamizu K, Watanabe M. Pulsed-gradient spin-echo 1H and 19F NMR ionic diffusion coefficient, viscosity, and ionic conductivity of non-chloroaluminate room-temperature ionic liquids. The Journal of Physical Chemistry B. 2001; 105(20):4603-4610
Freire MG, Neves CM, Marrucho IM, Coutinho JA, Fernandes AM. Hydrolysis of tetrafluoroborate and hexafluorophosphate counter ions in imidazolium-based ionic liquids. The Journal of Physical Chemistry A. 2009; 114(11):3744-3749
Gao H, Luo M, Xing J, Wu Y, Li Y, Li W, Liu Q, Liu H. Desulfurization of fuel by extraction with pyridinium-based ionic liquids. Industrial & Engineering Chemistry Research. 2008; 47(21):8384-8388. DOI: 10.1021/ie800739w
Kogelnig D, Stojanovic A, Galanski M, Groessl M, Jirsa F, Krachler R, Keppler BK. Greener synthesis of new ammonium ionic liquids and their potential as extracting agents. Tetrahedron Letters. 2008; 49(17):2782-2785
Pont A-L, Marcilla R, De Meatza I, Grande H, Mecerreyes D. Pyrrolidinium-based polymeric ionic liquids as mechanically and electrochemically stable polymer electrolytes. Journal of Power Sources. 2009; 188(2):558-563
Paduszyński K, Domańska U. Experimental and theoretical study on infinite dilution activity coefficients of various solutes in piperidinium ionic liquids. The Journal of Chemical Thermodynamics. 2013; 60:169-178
Breitbach ZS, Armstrong DW. Characterization of phosphonium ionic liquids through a linear solvation energy relationship and their use as GLC stationary phases. Analytical and Bioanalytical Chemistry. 2008; 390(6):1605-1617
Qian W, Texter J, Yan F. Frontiers in poly (ionic liquid)s: Syntheses and applications. Chemical Society Reviews. 2017; 46(4):1124-1159
Rojas MF, Bernard FL, Aquino A, Borges J, Dalla Vecchia F, Menezes S, Ligabue R, Einloft S. Poly (ionic liquid) s as efficient catalyst in transformation of CO2 to cyclic carbonate. Journal of Molecular Catalysis A: Chemical. 2014; 392:83-88
Hallett JP, Welton T. Room-temperature ionic liquids: Solvents for synthesis and catalysis. 2. Chemical Reviews. 2011; 111(5):3508-3576
Bara JE, Carlisle TK, Gabriel CJ, Camper D, Finotello A, Gin DL, Noble RD. Guide to CO2 separations in imidazolium-based room-temperature ionic liquids. Industrial & Engineering Chemistry Research. 2009; 48(6):2739-2751
Lei Z, Dai C, Yang Q, Zhu J, Chen B. UNIFAC model for ionic liquid-CO (H2) systems: An experimental and modeling study on gas solubility. AIChE Journal. 2014; 60(12):4222-4231
Gurkan BE, de la Fuente JC, Mindrup EM, Ficke LE, Goodrich BF, Price EA, Schneider WF, Brennecke JF. Equimolar CO2 absorption by anion-functionalized ionic liquids. Journal of the American Chemical Society. 2010; 132(7):2116-2117
Ruckart KN, O’Brien RA, Woodard SM, West KN, Glover TG. Porous solids impregnated with task-specific ionic liquids as composite sorbents. The Journal of Physical Chemistry C. 2015; 119(35):20681-20697
Wickramanayake S, Hopkinson D, Myers C, Hong L, Feng J, Seol Y, Plasynski D, Zeh M, Luebke D. Mechanically robust hollow fiber supported ionic liquid membranes for CO2 separation applications. Journal of Membrane Science. 2014; 470:52-59
Scovazzo P, Havard D, McShea M, Mixon S, Morgan D. Long-term, continuous mixed-gas dry fed CO2/CH4 and CO2/N2 separation performance and selectivities for room temperature ionic liquid membranes. Journal of Membrane Science. 2009; 327(1-2):41-48
Khan NA, Hasan Z, Jhung SH. Ionic liquids supported on metal-organic frameworks: Remarkable adsorbents for adsorptive desulfurization. Chemistry-A European Journal. 2014; 20(2):376-380
Vicent-Luna JM, Gutiérrez-Sevillano JJ, Anta JA, Calero S. Effect of room-temperature ionic liquids on CO2 separation by a Cu-BTC metal–organic framework. The Journal of Physical Chemistry C. 2013; 117(40):20762-20768
Li Z, Jia Z, Luan Y, Mu T. Ionic liquids for synthesis of inorganic nanomaterials. Current Opinion in Solid State and Materials Science. 2008; 12(1):1-8
Sheldon R. Catalytic reactions in ionic liquids. Chemical Communications. 2001; 23:2399-2407
Huddleston JG, Willauer HD, Swatloski RP, Visser AE, Rogers RD. Room temperature ionic liquids as novel media for ‘clean’ liquid–liquid extraction. Chemical Communications. 1998; 16:1765-1766
Enders Dickinson V, Williams ME, Hendrickson SM, Masui H, Murray RW. Hybrid redox polyether melts based on polyether-tailed counterions. Journal of the American Chemical Society. 1999; 121(4):613-616
Kubisa P. Application of ionic liquids as solvents for polymerization processes. Progress in Polymer Science. 2004; 29(1):3-12
Ngo HL, LeCompte K, Hargens L, McEwen AB. Thermal properties of imidazolium ionic liquids. Thermochimica Acta. 2000; 357:97-102
Bradley A, Hardacre C, Holbrey J, Johnston S, McMath S, Nieuwenhuyzen M. Small-angle X-ray scattering studies of liquid crystalline 1-alkyl-3-methylimidazolium salts. Chemistry of Materials. 2002; 14(2):629-635
Varma R. Solvent-free organic syntheses. Using supported reagents and microwave irradiation. Green Chemistry. 1999; 1(1):43-55
Davoodnia A, Heravi MM, Safavi-Rad Z, Tavakoli-Hoseini N. Green, one-pot, solvent-free synthesis of 1, 2, 4, 5-tetrasubstituted imidazoles using a Brønsted acidic ionic liquid as novel and reusable catalyst. Synthetic Communications. 2010; 40(17):2588-2597
Endres F, El Abedin SZ. Air and water stable ionic liquids in physical chemistry. Physical Chemistry Chemical Physics. 2006; 8(18):2101-2116
Bonhote P, Dias A-P, Papageorgiou N, Kalyanasundaram K, Grätzel M. Hydrophobic, highly conductive ambient-temperature molten salts. Inorganic Chemistry. 1996; 35(5):1168-1178
Carda–Broch S, Berthod A, Armstrong D. Solvent properties of the 1-butyl-3-methylimidazolium hexafluorophosphate ionic liquid. Analytical and Bioanalytical Chemistry. 2003; 375(2):191-199
Seddon KR, Stark A, Torres M-J. Influence of chloride, water, and organic solvents on the physical properties of ionic liquids. Pure and Applied Chemistry. 2000; 72(12):2275-2287
Susan MA, Noda A, Mitsushima S, Watanabe M. Brønsted acid–base ionic liquids and their use as new materials for anhydrous proton conductors. Chemical Communications. 2003; 8:938-939
Greaves TL, Weerawardena A, Fong C, Krodkiewska I, Drummond CJ. Protic ionic liquids: Solvents with tunable phase behavior and physicochemical properties. The Journal of Physical Chemistry B. 2006; 110(45):22479-22487
Mehrkesh A, Karunanithi A. Predicting Melting point and Viscosity of Ionic Liquids Using New Quantum Chemistry Descriptors. arXiv preprint arXiv:161200879. 2016
Cole AC, Jensen JL, Ntai I, Tran KLT, Weaver KJ, Forbes DC, Davis JH. Novel Brønsted acidic ionic liquids and their use as dual solvent-catalysts. Journal of the American Chemical Society. 2002; 124(21):5962-5963
Marsh K, Boxall J, Lichtenthaler R. Room temperature ionic liquids and their mixtures—A review. Fluid Phase Equilibria. 2004; 219(1):93-98
Tanaka K. In: Wasserscheid P, Welton T, editors. Ionic Liquids in Synthesis. Weinheim: Wiley-VCH; 2003. Wiley-VCH W. Search PubMed
Huddleston JG, Visser AE, Reichert WM, Willauer HD, Broker GA, Rogers RD. Characterization and comparison of hydrophilic and hydrophobic room temperature ionic liquids incorporating the imidazolium cation. Green Chemistry. 2001; 3(4):156-164
Schröder U, Wadhawan JD, Compton RG, Marken F, Suarez PA, Consorti CS, de Souza RF, Dupont J. Water-induced accelerated ion diffusion: Voltammetric studies in 1-methyl-3-[2,6-(S)-dimethylocten-2-yl] imidazolium tetrafluoroborate, 1-butyl-3-methylimidazolium tetrafluoroborate and hexafluorophosphate ionic liquids. New Journal of Chemistry. 2000; 24(12):1009-1015
MacFarlane D, Meakin P, Sun J, Amini N, Forsyth M. Pyrrolidinium imides: A new family of molten salts and conductive plastic crystal phases. The Journal of Physical Chemistry B. 1999; 103(20):4164-4170
Greaves TL, Drummond CJ. Protic ionic liquids: Properties and applications. Chemical reviews. 2008; 108(1):206-237
Nazari S, Cameron S, Johnson MB, Ghandi K. Physicochemical properties of imidazo-pyridine protic ionic liquids. Journal of Materials Chemistry A. 2013; 1(38):11570-11579
Irge DD. Ionic liquids: A review on greener chemistry applications, quality ionic liquid synthesis and economical viability in a chemical processes. American Journal of Physical Chemistry. 2016; 5:74-79
Duan X, Ma J, Lian J, Zheng W. The art of using ionic liquids in the synthesis of inorganic nanomaterials. CrystEngComm. 2014; 16(13):2550-2559
Kwon SG, Hyeon T. Formation mechanisms of uniform nanocrystals via hot-injection and heat-up methods. Small. 2011; 7(19):2685-2702
Cooper ER, Andrews CD, Wheatley PS, Webb PB, Wormald P, Morris RE. Ionic liquids and eutectic mixtures as solvent and template in synthesis of zeolite analogues. Nature. 2004; 430(7003):1012
Taubert A. CuCl Nanoplatelets from an ionic liquid-crystal precursor. Angewandte Chemie. 2004; 116(40):5494-5496
Antonietti M, Kuang D, Smarsly B, Zhou Y. Ionic liquids for the convenient synthesis of functional nanoparticles and other inorganic nanostructures. Angewandte Chemie International Edition. 2004; 43(38):4988-4992
Taubert A. Inorganic materials synthesis-a bright future for ionic liquids? Acta Chimica Slovenica. 2005; 52(3):183
Manojkumar K, Sivaramakrishna A, Vijayakrishna K. A short review on stable metal nanoparticles using ionic liquids, supported ionic liquids, and poly (ionic liquids). Journal of Nanoparticle Research. 2016; 18(4):1-22
Roucoux A, Schulz J, Patin H. Reduced transition metal colloids: A novel family of reusable catalysts? Chemical Reviews. 2002; 102(10):3757-3778
Sajjadi H, Modaressi A, Magri P, Domańska U, Sindt M, Mieloszynski J-L, Mutelet F, Rogalski M. Aggregation of nanoparticles in aqueous solutions of ionic liquids. Journal of Molecular Liquids. 2013; 186:1-6
Biswas K. Rao CeNeR. Use of ionic liquids in the synthesis of nanocrystals and nanorods of semiconducting metal chalcogenides. Chemistry–A European Journal. 2007; 13(21):6123-6129
Zhao X-L, Wang C-X, Hao X-P, Yang J-X, Wu Y-Z, Tian Y-P, Tao X-T, Jiang M-H. Synthesis of PbS nanocubes using an ionic liquid as the solvent. Materials Letters. 2007; 61(26):4791-4793
Tshemese Z, Mlowe S, Revaprasadu N, Deenadayalu N. Synthesis of CdS quantum dots in an imidazolium based ionic liquid. Materials Science in Semiconductor Processing. 2017; 71:258-262
Migowski P, Machado G, Texeira SR, Alves MC, Morais J, Traverse A, Dupont J. Synthesis and characterization of nickel nanoparticles dispersed in imidazolium ionic liquids. Physical Chemistry Chemical Physics. 2007; 9(34):4814-4821
Redel E, Walter M, Thomann R, Vollmer C, Hussein L, Scherer H, Krüger M, Janiak C. Synthesis, stabilization, functionalization and, DFT calculations of gold nanoparticles in fluorous phases (PTFE and ionic liquids). Chemistry-A European Journal. 2009; 15(39):10047-10059
Fonseca GS, Machado G, Teixeira SR, Fecher GH, Morais J, Alves MC, Dupont J. Synthesis and characterization of catalytic iridium nanoparticles in imidazolium ionic liquids. Journal of Colloid and Interface Science. 2006; 301(1):193-204
Wang Y, Yang H. Oleic acid as the capping agent in the synthesis of noble metal nanoparticles in imidazolium-based ionic liquids. Chemical Communications. 2006; 24:2545-2547
Salas G, Santini CC, Philippot K, Collière V, Chaudret B, Fenet B, Fazzini PF. Influence of amines on the size control of in situ synthesized ruthenium nanoparticles in imidazolium ionic liquids. Dalton Transactions. 2011; 40(17):4660-4668
Duan X, Kim T, Li D, Ma J, Zheng W. Understanding the effect models of ionic liquids in the synthesis of NH4-Dw and γ-AlOOH nanostructures and their conversion into porous γ-Al2O3. Chemistry-A European Journal. 2013; 19(19):5924-5937
Duan X, Li D, Zhang H, Ma J, Zheng W. Crystal-facet engineering of ferric Giniite by using ionic-liquid precursors and their enhanced Photocatalytic performances under visible-light irradiation. Chemistry-A European Journal. 2013; 19(22):7231-7242
Ding K, Miao Z, Liu Z, Zhang Z, Han B, An G, Miao S, Xie Y. Facile synthesis of high quality TiO2 nanocrystals in ionic liquid via a microwave-assisted process. Journal of the American Chemical Society. 2007; 129(20):6362-6363
Zheng W, Liu X, Yan Z, Zhu L. Ionic liquid-assisted synthesis of large-scale TiO2 nanoparticles with controllable phase by hydrolysis of TiCl4. ACS Nano. 2008; 3(1):115-122
Liu X, Ma J, Zheng W. Applications of ionic liquids (ILs) in the convenient synthesis of nanomaterials. Reviews on Advanced Materials Science. 2011; 27:43-51
Alavi-Tabari SA, Khalilzadeh MA, Karimi-Maleh H. Simultaneous determination of doxorubicin and dasatinib as two breast anticancer drugs uses an amplified sensor with ionic liquid and ZnO nanoparticle. Journal of Electroanalytical Chemistry. 2018; 811:84-88
Husanu E, Chiappe C, Bernardini A, Cappello V, Gemmi M. Synthesis of colloidal Ag nanoparticles with citrate based ionic liquids as reducing and capping agents. Colloids and Surfaces A: Physicochemical and Engineering Aspects. 2018; 538:506-512
Shang W, Cai T, Zhang Y, Liu D, Sun L, Su X, Liu S. Covalent grafting of chelated othoborate ionic liquid on carbon quantum dot towards high performance additives: Synthesis, characterization and tribological evaluation. Tribology International. 2018; 121:302-309
Saien J, Hashemi S. Long chain imidazolium ionic liquid and magnetite nanoparticle interactions at the oil/water interface. Journal of Petroleum Science and Engineering. 2018; 160:363-371
Okoli CU, Kuttiyiel KA, Cole J, McCutchen J, Tawfik H, Adzic RR, Mahajan D. Solvent effect in sonochemical synthesis of metal-alloy nanoparticles for use as electrocatalysts. Ultrasonics Sonochemistry. 2018; 41:427-434
Sotolongo AC, Martinis EM, Wuilloud RG. An easily prepared graphene oxide–ionic liquid hybrid nanomaterial for micro-solid phase extraction and preconcentration of Hg in water samples. Analytical Methods; 2018; 10:338-346
Lu J, Yang J-X, Wang J, Lim A, Wang S, Loh KP. One-pot synthesis of fluorescent carbon nanoribbons, nanoparticles, and graphene by the exfoliation of graphite in ionic liquids. ACS Nano. 2009; 3(8):2367-2375
Wang B, Song A, Feng L, Ruan H, Li H, Dong S, Hao J. Tunable amphiphilicity and multifunctional applications of ionic-liquid-modified carbon quantum dots. ACS Applied Materials & Interfaces. 2015; 7(12):6919-6925
Tan Y, Li M, Ye X, Wang Z, Wang Y, Li C. Ionic liquid auxiliary exfoliation of WS2 nanosheets and the enhanced effect of hollow gold nanospheres on their photoelectrochemical sensing towards human epididymis protein 4. Sensors and Actuators B: Chemical. 2018; 262:982-990
Prechtl MH, Campbell PS, Scholten JD, Fraser GB, Machado G, Santini CC, Dupont J, Chauvin Y. Imidazolium ionic liquids as promoters and stabilising agents for the preparation of metal (0) nanoparticles by reduction and decomposition of organometallic complexes. Nanoscale. 2010; 2(12):2601-2606
Kohler N, Sun C, Wang J, Zhang M. Methotrexate-modified superparamagnetic nanoparticles and their intracellular uptake into human cancer cells. Langmuir. 2005; 21(19):8858-8864
Bertorelle F, Wilhelm C, Roger J, Gazeau F, Ménager C, Cabuil V. Fluorescence-modified superparamagnetic nanoparticles: Intracellular uptake and use in cellular imaging. Langmuir. 2006; 22(12):5385-5391
Shenhar R, Norsten TB, Rotello VM. Polymer-mediated nanoparticle assembly: Structural control and applications. Advanced Materials. 2005; 17(6):657-669
Mohan B, Woo H, Jang S, Lee S, Park S, Park KH. Synthesis of monodisperse cu nanoparticles in ionic liquids: A synthetic and catalytic approach of in situ nanoparticles. Solid State Sciences. 2013; 22:16-20
Kim K-S, Demberelnyamba D, Lee H. Size-selective synthesis of gold and platinum nanoparticles using novel thiol-functionalized ionic liquids. Langmuir. 2004; 20(3):556-560
Gracia R, Vijayakrishna K, Mecerreyes D. Poly (ionic liquid) s with redox active counter-anions: All-in-one reactants and stabilizers for the synthesis of functional colloids. Reactive and Functional Polymers. 2014; 79:54-58
Vijayakrishna K, Charan K, Manojkumar K, Venkatesh S, Pothanagandhi N, Sivaramakrishna A, Mayuri P, Kumar AS, Sreedhar B. Ni nanoparticles stabilized by poly (ionic liquids) as chemoselective and magnetically recoverable catalysts for transfer hydrogenation reactions of carbonyl compounds. ChemCatChem. 2016; 8(6):1139-1145
Tshemese Z, Khan MD, Mlowe S, Revaprasadu N. Synthesis and characterization of PbS nanoparticles in an ionic liquid using single and dual source precursors. Materials Science and Engineering: B. 2018; 227:116-121